# Modeling linear and nonlinear soft ferromagnetic materials

Full text

(2)

(3) Als meus pares, Josep Sebasti`a i Empar, i a la mem`oria dels meus iaios, Justo i Jos´e..

(4)

(5) Preface. Today magnets form part of our daily life. They are responsible for most of the energy generation (e.g. turbines), conversion (e.g. transformers) and its use (e.g. motors). In these applications the precise control of magnetic fields and magnetization is essential to devise new applications or to improve the existing ones. All these would not be possible without an impressive development of magnetic materials. For example, in the last century very large (hard magnets) and very small (soft magnets) values of crystalline anisotropy have been achieved, spanning in five orders of magnitude. The vast range of coercivities makes possible the design of the shape of the hysteresis loop desired for a particular application. Soft ferromagnets are of great interest because they can guide and concentrate magnetic fields and present low hysteresis and large values of both saturation magnetization and susceptibility. These materials are found, for instance, in electromagnets, where a soft ferromagnetic core is set to concentrate the field, and in electrical transformers, motors or generators, in which the low power loss is an advantage. The large number of existing and potential applications of soft ferromagnets ranges from large scales (meters) to very small scales (nanometers). One of the large scale applications is superconducting magnetic levitation. Superconductors have demonstrated to present stable and passive levitation lifting weights of hundreds of kilograms. Using these concepts, superconducting materials can be located in a vehicle that levitates above a permanent-magnet guideway in what is known a magnetic levitation vehicle. The main advantage of this technology is its contactless nature which allows a major reduction of friction, and therefore larger vehicle speeds can be achieved with the same power consumption. Soft ferromagnets located in the guideway modify the magnetic field landscape of the permanent magnets leading to optimized values of levitation force and stability of the levitating superconducting vehicle. At the small scale, a very important application of soft ferromagnets is in magnetic recording and since few decades ago, this industry has been pushing hard in the deep understanding of magnetism at the nanoscale. In essence magnets produce magnetic 3.

(6) 4 fields that can be used to store bits of information. This information can be read using a magnetoresistive read head that consists of a multilayer of soft ferromagneticmetal-soft ferromagnetic with one of the ferromagnetic layers (pinned layer) attached to an antiferromagnet. The other ferromagnetic layer is free to sense the magnetic field at very small spatial scales. Information can also be stored in arrays of magnetic tunnel junctions or simply cylindrical soft ferromagnets. These latter ones can present a magnetic vortex state at remanence, a magnetization pattern that can store two bits of information increasing the information density (number of bits per area of magnetic media). The aim of the present thesis is to model the behavior of soft ferromagnets in the macroscopic and microscopic scales and their interaction with other magnetic materials such as permanent magnets, superconductors or antiferromagnets for their use in the mentioned applications. This thesis is structured in two parts. In Part I we introduce a model that describes the mutual interaction of a linear, isotropic, and homogeneous soft ferromagnetic bar with a hard type II superconductor. The model is applied to the optimization of a typical magnetic levitation guideway. In Part II a non linear model based on micromagnetic scheme is introduced to model soft ferromagnets at the nanoscale range. The model is applied to the study of exchange biased systems and the control of magnetic vortex states. Before starting with the first part, we review in the first chapter the main concepts used throughout the thesis, introducing the main characteristics of ferromagnetic materials and the critical-state model, a model widely accepted in the description of the macroscopic behavior of a hard type II superconductor, which we will use. In the first part (Chapter 2) we start by reviewing the properties that make superconductors good candidates to achieve a passive and static levitation. In Chapter 3 we introduce the model of a linear, isotropic, and homogeneous soft ferromagnet in the limit of very large susceptibility interacting with a superconductor. The magnetic poles in the ferromagnet and the currents induced in the superconductor will be calculated using a functional related to their magnetic energy. An advantage of the model presented is that both elements will mutually interact so that the magnetic pole density of the ferromagnet will be affected by the currents induced in the superconductor and vice versa. A systematic study of the soft ferromagnet will be performed in Chapter 4. The magnetic pole density in the ferromagnet will be studied when submitted to different applied fields. The first, a uniform applied field, is used to understand the basic phenomena and to compare our results with the existing analytical ones. Then the magnetic response of the ferromagnet in the fields produced by one or two magnets (non-uniform) is studied. The results of this chapter will be helpful to determine the size and shape that a soft ferromagnet must have in each of the three applied fields to enhance the magnetic field in a certain region of the space. In a Chapter 5 we use the results obtained in the previous chapter to maximize the.

(7) 5 levitation force and stability of a typical magnetic levitation system based on superconductors. Results in this chapter may be useful when designing future magnetic levitation systems. At the beginning of Part II we set the motivation for the study of magnetism at the nanoscale, and in particular we review the importance of soft ferromagnets in devices using giant magnetoresistance and magnetic memories. The model for a non-linear ferromagnet in the micromagnetic framework is presented in Chapter 6. In Chapter 7 we present the hysteretic behavior of a ferromagnetic cylinder at the nanoscale. Typically, the most stable magnetic configuration for this shape and size in a soft ferromagnet is the magnetic vortex state. A simple procedure is introduced to achieve independent control of chirality and polarity of a vortex state by simply adjusting the applied field direction given a particular dot geometry. An extension of the model presented in Chapter 6 is made in Chapter 8 to take into account the effect that an antiferromagnetic material makes to the macroscopic behavior of a soft ferromagnet. In this case, we will reproduce the basic phenomena of exchange bias and study the distortion that a magnetic vortex state suffers along the thickness of the soft ferromagnet due to the surface interaction with the antiferromagnet. Finally, in Chapter 9 the conclusions of this thesis and future lines are presented..

(8)

(9) Contents. 1 Basic Concepts in Magnetism 1.1 Magnetostatics and Magnetic Materials . . . . . . . . . . . . . . . . . . 1.1.1 Magnetic Moment and Magnetization . . . . . . . . . . . . . . . 1.1.2 Maxwell’s Static Equations: Magnetostatics . . . . . . . . . . . . 1.1.3 Magnetostatics without Free Currents . . . . . . . . . . . . . . . 1.1.4 Magnetic Susceptibility and Linear Isotropic and Homogeneous Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1.5 Demagnetizing Fields and Demagnetizing Factors . . . . . . . . . 1.2 Special Cases of Linear Isotropic and Homogeneous Magnetic Materials 1.2.1 χ → ∞ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2.2 χ → 0+ . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Ferromagnetic Materials . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4 Hard Superconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.4.1 Critical-State Model . . . . . . . . . . . . . . . . . . . . . . . . .. 11 11 11 12 12. I. Modeling Linear Soft Ferromagnets: Application to Levitation. 21. 2 Superconducting-Ferromagnetic Hybrids 2.1 Magnetic Levitation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Levitation with Diamagnets and Hard Type II Superconductors . . . . .. 23 23 24. 3 Numerical Model for Magnetic Interaction 3.1 Geometry and Magnetic Elements . . . . . 3.2 Interaction Functional . . . . . . . . . . . . 3.3 Calculation of Currents and Magnetic Poles 3.4 Calculation of Levitation Force . . . . . . . 3.5 Calculation of Stability . . . . . . . . . . . .. 27 27 28 30 32 32. 7. between SC . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. and . . . . . . . . . . . . . . .. FM . . . . . . . . . . . . . . .. . . . . .. . . . . .. 13 13 14 14 15 16 17 18.

(10) 8. CONTENTS 3.6. Limits and Validity of the Model . . . . . . . . . . . . . . . . . . . . . .. 4 Magnetic Response of an Ideal Soft Ferromagnet 4.1 Uniform Applied Field . . . . . . . . . . . . . . . . 4.2 Permanent-Magnet field . . . . . . . . . . . . . . . 4.3 Two Permanent-Magnets Field . . . . . . . . . . . 4.4 Chapter Summary and Conclusions . . . . . . . . .. . . . .. . . . .. . . . .. 5 Optimization of a Superconducting Levitation System 5.1 Geometry for High Levitation Force . . . . . . . . . . . 5.2 General Effect of a Soft Ferromagnet in Levitation . . . 5.3 Stability and Minor Loops . . . . . . . . . . . . . . . . . 5.4 Optimization of the Ferromagnet Width . . . . . . . . . 5.5 Modifying the Permanent Magnet Width . . . . . . . . 5.6 Chapter Summary and Conclusions . . . . . . . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. . . . .. . . . . . .. 33. . . . .. 35 35 37 40 42. . . . . . .. 43 43 45 48 52 54 55. II Modeling Magnetism at the Nanoscale: Application to Exchange Bias and Thin Soft Ferromagnets 57 6 Micromagnetic Model 6.1 Micromagnetic Energy Density and Assumptions 6.2 Brown’s Static Equations . . . . . . . . . . . . . 6.3 Discretization of Effective Field . . . . . . . . . . 6.3.1 Applied Field . . . . . . . . . . . . . . . . 6.3.2 Uniaxial Anisotropy Field . . . . . . . . . 6.3.3 Exchange Field . . . . . . . . . . . . . . . 6.3.4 Magnetostatic or Stray Field . . . . . . . 6.4 Numerical Iterative Procedure . . . . . . . . . . . 6.5 Limits and Validity of the Model . . . . . . . . . 7 Geometrical Control of Magnetic Vortex States 7.1 Submicrometer Dot Hysteresis Loop . . . . . . . 7.2 Thickness-Modulated Ferromagnetic Dot . . . . . 7.3 Analytical Model . . . . . . . . . . . . . . . . . . 7.4 Chapter Summary and Conclusions . . . . . . . .. . . . . . . . . .. . . . .. . . . . . . . . .. . . . .. . . . . . . . . .. . . . .. 8 Exchange Bias in Cylindrical Nanomagnets 8.1 Exchange Bias Phenomenology and Existing Models . 8.2 Modeling Exchange Bias in Micromagnetic Formalism 8.3 Distortion of an Exchange Biased Vortex . . . . . . . . 8.4 Effect on the Antiferromagnet Thickness . . . . . . . . 8.5 Chapter Summary and Conclusions . . . . . . . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. . . . .. . . . . .. . . . . . . . . .. 61 61 62 64 64 64 65 66 68 69. . . . .. 71 72 74 79 81. . . . . .. 83 83 85 87 92 93.

(11) CONTENTS. 9. 9 Conclusions of the Work and Future Lines A Geometrical Factors for Magnetic Scalar Potential and Magnetic tor Potential A.1 Magnetic Scalar Potential Over the FM . . . . . . . . . . . . . . . . A.1.1 Calculation of the Matrices Eij . . . . . . . . . . . . . . . . . A.1.2 Calculation of Matrices QSC ij . . . . . . . . . . . . . . . . . . . A.2 Potential Vector Over the SC . . . . . . . . . . . . . . . . . . . . . . A.2.1 Calculation of Matrices Di,j . . . . . . . . . . . . . . . . . . . A.2.2 Calculation of Matrices QFM . . . . . . . . . . . . . . . . . . ij. 95 Vec. . . . . .. . . . . . .. Appendices B Magnetostatic Field Interaction Matrix . . . . . . . . . . . . . . . . . . . C Solution of Standard Problem # 2 . . . . . . . . . . . . . . . . . . . . . Bibliography . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 99 99 99 101 102 102 103. 98 105 109 113.

(12)

(13) CHAPTER. 1. Basic Concepts in Magnetism. In this chapter we review the basic concepts used in this thesis. In the first part we present the main physical quantities describing the magnetism of materials. In the second section we briefly explain ferromagnetism and the energies involved. Finally, we introduce the main properties of superconducting materials and present a macroscopic model that describes the magnetic behavior of hard superconductors.. 1.1. Magnetostatics and Magnetic Materials. A magnetic material is a material that produces a magnetic field either spontaneous or when submitted to an external applied field. In this section we review some key concepts involving the magnetism of materials.. 1.1.1. Magnetic Moment and Magnetization. In classical magnetostatics the dipolar magnetic moment created by a current density J is Z 1 r × J(r)dV, (1.1) m= 2 where V is the volume where the current is present. In magnetic materials, apart from the magnetic dipole induced by the currents flowing through it, there is an intrinsic magnetic moment of quantum mechanical origin associated with the spin (angular momentum) of each electron [1, 2]. In materials where the spins locally point in the same direction we can define the magnetization vector M which is a mesoscopic volume average of the magnetic moments M(r) = dm/dV . The macroscopic volume average magnetization of a sample either from currents or magnetic moments is defined by R Mvol ≡ mdV /Vs where Vs is the volume of the sample. 11.

(14) 12. 1.1.2. Basic Concepts in Magnetism. Maxwell’s Static Equations: Magnetostatics. When no magnetic moments or currents vary on time, the two fundamental equations in magnetostatics are ∇ × H = J,. (1.2). ∇ · B = 0,. (1.3). where H is the magnetic field, B is the magnetic induction and J is the free current density [3]. The boundary conditions of the magnetic induction and the magnetic field between two magnetic materials are (H1 − H2 ) × en = 0,. (1.4). (B1 − B2 ) · en = 0,. (1.5). where 1 and 2 indicate the magnetic medium and en the unit vector perpendicular to the interface pointing from medium 1 to 2. The quantity that relates magnetic induction and magnetic field is the magnetization according to B = µ0 (H + M) ,. (1.6). where µ0 is the vacuum permeability. The divergenceless nature of the magnetic induction [see Eq. (1.3)] which is also accomplished in the non-static regime allows the definition of a magnetic vector potential A(r) such that B(r) = ∇ × A(r).. (1.7). The choice of ∇ · A(r) or gauge is free since it does not change B(r). A common gauge used is the Coulomb gauge ∇ · A(r) = 0.. 1.1.3. Magnetostatics without Free Currents. In magnetic materials where the free current density is zero (J=0) Eqs. (1.2), (1.3), (1.4) and (1.5) can be rewritten as ∇ × H = 0, ∇ · H = ρM , (H1 − H2 ) × en = 0, (H1 − H2 ) · en = −σM ,. (1.8) (1.9) (1.10) (1.11). where ρM and σM are the volume and surface magnetic pole densities, respectively and are defined as ρM ≡ −∇ · M,. (1.12). σM ≡ (M1 − M2 ) · en .. (1.13).

(15) 1.1 Magnetostatics and Magnetic Materials. 13. Equations (1.9) and (1.11) along with Eqs. (1.12) and (1.13) indicate that the source of magnetic field is due to a variation of the magnetization either in the volume [Eq. (1.12)] or in the surface sample [Eq. (1.13)]. Magnetic field lines start in positive magnetic poles and end in negative magnetic poles but never forming a closed loop. The vanishing curl of H(r) in current free magnetic materials allows the definition of the magnetic scalar potential φ, whose gradient is H(r) = −∇φ(r). This potential is enough to describe the magnetic field in the whole space.. 1.1.4. Magnetic Susceptibility and Linear Isotropic and Homogeneous Materials. Magnetization M at each point in the sample is related to the magnetic field H in the same point as M(r) = χ(H, r)H(r), (1.14) where χ(H, r) is an intrinsic parameter of the magnetic material known as the magnetic susceptibility. In general, χ is a tensor that depends on the position r and the local field H(r) inside the material. A linear isotropic and homogeneous material (LIH) is defined as a material for which χ is a scalar quantity (isotropic) independent of the field (linear) and the position (homogeneous) so that M(r) = χH(r),. (1.15). is accomplished being χ is a real quantity. A LIH material can also be characterized by the magnetic permeability µ which is related to the susceptibility as µ χ= − 1. (1.16) µ0 In a LIH material without any free current the combination of Eqs. (1.3), (1.6), (1.12) and (1.15) leads to the conclusion that no volumic poles are induced and therefore the divergence of H vanishes inside the sample. Only the difference (divergence) of M at the surface induce a surface magnetic pole density according to Eq. (1.13). Another characteristic of this approximation (LIH) is that no irreversible processes can be described.. 1.1.5. Demagnetizing Fields and Demagnetizing Factors. The magnetic behavior of a sample does not only depend on its intrinsic properties such as χ(H, r) but on the shape of the magnetic sample itself [4, 5]. This can be understood by looking at the boundary conditions Eqs. (1.4) and (1.5). The geometrical effects of the magnetic sample are usually called demagnetizing effects. The demagnetizing field Hd or stray field is the magnetic field generated by the surface and volumic magnetic pole densities in a magnet. If an external magnetic field Ha is applied to the sample, the total magnetic field at any point in the space is H = Ha + Hd .. (1.17).

(16) 14. Basic Concepts in Magnetism. The averaged volume magnetization of a sample is related to the averaged volume demagnetizing field Hd,vol as Hd,vol = −N Mvol , (1.18) where N is the magnetometric demagnetizing tensor. In general, Hd,vol and Mvol are not parallel even in LIH materials. In some cases, as for instance LIH ellipsoidal samples this two quantities are strictly parallel and the demagnetizing tensor reduces to a scalar quantity called demagnetizing factor which can be defined as N =−. Hd,vol . Mvol. (1.19). In general, the directions of Ha for which all the averaged magnetic quantities are parallel and the demagnetizing tensor is reduced to a scalar are called the principal directions of the sample. In this case, the demagnetizing tensor [defined in Eq. 1.18] expressed in the basis of the principal directions is diagonal. i.e. has zeros in the non-diagonal part of the matrix.. 1.2. Special Cases of Linear Isotropic and Homogeneous Magnetic Materials. The demagnetizing fields for LIH materials with χ → 0+ and χ → ∞ are analyzed in this section.. 1.2.1. χ→∞. When a uniform field is applied to a sample of positive susceptibility, the average volume magnetization Mvol has the same direction as the external uniform applied field Ha , as shown in Fig. 1.1(a). Positive magnetic pole density is generated in the surface whose normal vector (directed outwards the sample) has the same direction as the applied field. Conversely a negative surface magnetic pole density appears when the normal to the surface is antiparallel to the field as indicated by Eq. (1.13). As seen in Figs. 1.1(a) and 1.1(b) for χ > 0 the magnetic field produced by the poles in the interior of the sample is opposite to the averaged magnetization direction. Therefore, the total magnetic field inside the sample H = Ha + Hd is reduced with respect to the applied field. The fact that Hd reduces the magnetic field inside the sample gives the original name of demagnetizing field to Hd . When χ → ∞, we can see by the definition of magnetic susceptibility Eq. (1.14) that H inside the sample must be zero so that the magnetization M remains finite. This implies that inside the sample the demagnetizing field is the same but with opposite direction to the applied field, i.e. Hd = −Ha as depicted in Fig. 1.1(a). In this case, since the total magnetic field inside the sample is zero (this is, H1 = 0), the perpendicular boundary condition [Eq. (1.11)] indicates that at the surface of the sample the field takes a value |H| = σM . No magnetic field component parallel to the surface exists [Eq. (1.10).

(17) 1.2 Special Cases of Linear Isotropic and Homogeneous Magnetic Materials. (a). 15. (b). Mvol. M. Ha. Figure 1.1: Surface magnetic pole density indicated by signs and demagnetizing field lines (dashed) for two LIH materials, χ → ∞ (a) and χ =→ 0+ (b).. and H1 = 0] and therefore the magnetic field at the surface is perpendicular to it with expression H = σM en . In magnetically soft materials (large χ) the initial slope of a hysteresis loop far from saturation is very large and almost linear. For instance the typical slope for Permalloy material is 105 . The approximation of χ → ∞ is only valid in this kind of materials and in the applied field region where the material is far from saturation.. 1.2.2. χ → 0+. The limit of vanishing χ (from positive values) describes well the saturated regime of ferromagnetic materials. This is, in the limit where the magnetization does not change due to an increment or decrement of the applied magnetic field. It is also a way to describe permanent magnets (PMs), or magnetic materials that due to their intrinsic properties are magnetized mostly in one direction and do not change their magnetization in a large range of applied magnetic fields. A typical example of a permanent magnetic material is NdFeB having huge coercivities about 2.5 Tesla [6]. In the uniform magnetization or, equivalently χ = 0 limit, the magnetic pole density is constant on the surfaces perpendicular to the applied field as shown in Fig. 1.1(b). In this case, even though the magnetization is constant in the sample volume the demagnetizing field is not uniform. This apparent contradiction is solved as follows. For small χ the magnetization of the sample is small according to Eq. (1.14) and therefore small magnetic pole density is generated resulting in a small demagnetizing field. Since H = Ha + Hd a small uniform applied field Ha >> Hd will make that inside the material the magnetic field H is in the direction of Ha . Therefore the magnetization has the same uniform direction as the applied field according to M = χH..

(18) 16. 1.3. Basic Concepts in Magnetism. Ferromagnetic Materials. Even though we can consider magnetic materials as LIH in some cases (explained above), in general they present an irreversible behavior as described by the hysteresis loops. Ferromagnetic materials [2, 7] at a temperature below its Curie temperature Tc (temperature above which the ferromagnetic ordering no longer exists) may present small zones called magnetic domains in which the magnetization remains mostly in one direction. The existence of domains was proposed by Weiss back in the year 1907 in order to explain why materials known to be ferromagnetic did not have a net magnetic moment at the macroscopic scale [8]. The irreversible processes in a ferromagnet (FM) occur due to coherent rotation of the magnetization in a domain or by domain wall displacements. The study of these effects is complicated due to the high non linearity of the problem. Magnetic domains result from the competition of the main three energies in a FM: the magnetostatic, the exchange and the crystalline anisotropy energies. The magnetostatic energy results from the divergence of the magnetization, or in other words, the magnetic pole densities in a FM. This energy can be written as [1] Z 1 Ed = − µ0 Hd MdV. (1.20) 2 The minimization of the magnetostatic energy is achieved by reducing the magnetic poles (which is known as the magnetic pole avoidance principle [9]) or equivalently the demagnetizing field inside the sample. The exchange energy has a quantum origin [1, 10]. It reflects the competition between the Coulomb interaction of two nearby electrons, and the Pauli exclusion principle. This is, electrons in the same place can not have the same spin direction. If the Coulomb interaction is weak two electrons are close and therefore must point in opposite directions, conversely if the Coulomb interaction is strong they can point in the same direction. Heisenberg set up to express the Hamiltonian of this interaction for two spins as [2], H = −2JS1 · S2 ,. (1.21). where J is the exchange integral and S1 , S2 are dimensionless quantum operators. In the case of ferromagnetic materials J > 0 and neighboring spins point in the same direction. Ferromagnetic materials present, independently of their shape, directions of easy magnetization [7]. This is, a direction for which saturating the magnetic sample needs for a weaker applied field compared to other directions. This phenomenon is known as the crystalline anisotropy and is related with the crystal structure of the FM. A material with uniaxial crystalline anisotropy has two easy directions and its energy density can be expressed as E = K sin2 θ, (1.22) as a first approximation. Here, K is the anisotropy constant with units of J/m3 and θ = 0 or θ = π are the easy directions..

(19) 1.4 Hard Superconductors. 17. In soft materials (where the anisotropy is negligibly small) magnetostatic and exchange energies act on different scales to form domains. The main point is that the exchange energy density is several orders of magnitude larger than the magnetostatic one. However the magnetostatic energy density is of long range order whereas the exchange interaction is short range (neighboring spins). In this way, when the magnetic sample is large it forms domains where locally the exchange energy is minimized (spins point in the same direction) and globally the non uniformity of the domains reduces the magnetic pole density lowering the magnetostatic energy. Conversely, when the sample is small, the exchange forces dominate and the sample is uniformly magnetized approaching the limit χ = 0. Using these concepts, Brown announced what would be known as the fundamental theorem of fine particle theory [11]: the state of the lowest free energy of a ferromagnetic particle is one uniform magnetization if the particle is sufficiently small and one of nonuniform magnetization if it is sufficiently large. Size effects (not the shape) on a soft fine magnetic particle are studied briefly in Appendix C.. 1.4. Hard Superconductors. In this section we briefly review some of the main properties of the superconductors (SCs); readers are referred to [12, 13, 14, 15] for a further and deeper understanding of these materials. The superconducting state is a thermodynamic state of some materials that when cooled below a critical temperature Tcrit present two phenomena simultaneously. The first is that the electrical resistance drops abruptly to zero. The second is that for sufficiently low fields the SC presents perfect diamagnetism, this is, the field produced by the material is opposed to that of the applied field leading to null magnetic field intensity in the interior of the sample. Two aspects must be distinguished from the diamagnetic behavior of the SC. The first is the flux exclusion: when the SC is cooled below Tcrit at zero field and then a field is applied, the magnetic flux does not penetrate the sample. The second is the flux expulsion: cooling the SC in the presence of an applied field makes the magnetic flux to be expelled from the SC as it reaches the SC state. This last effect is known as the Meissner effect. Another fact worth mentioning from SC is that contrary to many magnetic materials in which the source of magnetic field is due to localized magnetic moments in the crystal (dipolar moment due to the angular momentum of the electrons), the SC magnetic response is due to a free current induced in the material. There are two types of SCs, type I and type II. Type I presents a Meissner state if the applied field Ha is below a critical field Hc specific for each material. In this type of SC some currents (shielding currents) flowing in a shell of depth λ (penetration depth) are induced in the surface of the SC in order to shield the magnetic induction inside it. So B is zero in all the sample volume but in the regions where currents penetrate. Type II SCs have the same properties as type I for any applied field below a certain.

(20) 18. Basic Concepts in Magnetism. critical value Hc,1 . However, between Hc,1 and another larger critical field Hc,2 (Hc,2 > Hc,1 ), magnetic induction partially penetrate inside the material bulk in the form of superconducting current vortices, a state commonly known as the mixed state. These vortices are quantized in the sense that each of them is surrounded by a current loop whose magnetic flux φ = h/2e = 2.07 · 10−15 Wb is quantized. In type II SC in the mixed state, current vortices repel each other due to the interaction of their magnetic induction generated. As a result, the vortices in a perfect type II SC distribute in a triangular array called the Abrikosov net [16]. Normally, SCs contain defects or impurities that can pin vortices, this is, they can keep a vortex fixed in a position with a force called the pinning force. These imperfections can compensate the repulsion of the vortices and suppress the Abrikosov net generating a non uniform distribution of vortices in the SC. This, at the same time makes a non-uniform distribution of B in some regions of the SC and according to Eq. (1.2) a macroscopic current density appears. The magnitude of the current density in these regions is limited by the average maximum pinning force, called critical-current density Jc . The type II SCs in the mixed state presenting a strong pinning force are commonly known as hard SCs.. 1.4.1. Critical-State Model. The critical-state model is a macroscopic model that describes the magnetic response of hard SCs. It was proposed by C. P. Bean [17, 18] and is based on the assumption that any electromagnetic force, whatever small, will induce a macroscopic constant current density Jc . This model applicability has been proved to be very broad to understand magnetic measurements [19, 20, 21, 22, 23, 24, 25, 26]. The critical-state model implicitly assumes that Hc,1 = 0, this is, no surface currents generated in the Meissner state are considered. In the following we review the main features of the Bean’s critical-state model by studying an example. We consider the case of an infinite slab 1 of hard SC immersed in a uniform applied field Ha in the y direction (this slab is finite in the x direction.). The SC is initially zero-field cooled below Tcrit . When the applied field is increased from zero some currents will be induced from the edge inwards following the Lenz’s law [3] as shown in Fig. 1.2(a). These currents are opposite in sign so that they try to shield SC volume. According to the model, the current density has a constant value Jc and since Jc = |∇ × H| = |∂Hy /∂x|, the total magnetic field inside the sample decays linearly. This is, at the edge of the sample H = Ha and decreases linearly up to zero. Two regions can be observed here, the region where the current has penetrated and therefore a non-zero magnetic field exists and a region where there is no current and consequently a vanishing magnetic field. If the applied field is further increased the SC currents penetrate even more inside the sample [Fig. 1.2(b)] up to a field Hp for which the sample is fully penetrated [Fig. 1. An infinite slab is a geometry consisting on two infinite directions and a finite one being the sides of the latter parallel and flat.

(21) 1.4 Hard Superconductors. 19. Figure 1.2: Sketch of current and field profiles within the Bean model for infinite slab in which the field is applied in the y direction (one of the infinite directions of the slab).. 1.2(c)]. Larger fields than Hp do not induce new currents in the sample but shift the total field at the interior of the sample as shown in Fig. 1.2(d). If the applied field is decreased after a maximum applied field Hm , critical-current density is induced in the opposite direction [Fig. 1.2(e)]. These currents, penetrate in the same way as the initial ones, this is, from the edges to the interior of the sample keeping the already existing currents frozen. The above example evidences the hysteretic nature of the critical-state model because, for instance, the initial state of zero applied field [Fig. 1.2(a)] is different to the state found at the same field after increasing and decreasing it as shown in Fig. 1.2(f). Even though we have solved the simplest case, critical-state modeling for different geometries such as cylinders or infinitely long bars has been solved and are reviewed in [27]..

(22)

(23) Part I. Modeling Linear Soft Ferromagnets: Application to Levitation. 21.

(24)

(25) CHAPTER. 2. Superconducting-Ferromagnetic Hybrids. The study of the interaction between soft ferromagnetic materials and superconductors has become an active topic of research because of their potential applications when properly combined. One of the areas that has attracted much attention is hightemperature coated conductors (CCs) [28, 29, 30] where usually [29] the superconducting material is deposited over a ferromagnetic substrate [31]. CCs are combined with soft ferromagnetic materials for electric and power applications such as high magnetic field generation [32], energy storage [33, 34, 35], motors [36] or fault current limiters [37] or even space gyroscopes [38]. For these applications a large critical-current density Jc and low AC losses (hysteretic losses) are advisable. Usually Jc is increased by adding some defects [39] to the SC that pin the vortices, however new studies reveal that soft ferromagnetic parts placed inside [40] or outside [41, 42, 43, 44, 45, 46, 47] the SC can increase its Jc . This effect is produced by the reduction of the magnetic field inside the SC, a result that can also be used to reduce the AC losses in SC cables [48, 49] and increase their transport current. Another important application of systems where superconductors and ferromagnets appear together is in levitation. In the following sections of this chapter we explain the concept of levitation and the usefulness of superconductors combined with soft ferromagnets for this application.. 2.1. Magnetic Levitation. Levitation is the process by which an object or body is suspended by a force against gravity remaining in a stable position without contact. There are many forces on the nature that can make an object to levitate [50] and depending on their nature can be: aerodynamic (produced by gas pressure), acoustic (sound pressure), electrostatic 23.

(26) 24. Superconducting-Ferromagnetic Hybrids. (electric fields) or magnetic (magnetic fields), among others. In this section we will analyze magnetic levitation. A levitation system must be stable, this is, if the levitating object is slightly displaced from its equilibrium position there must exist some restoring forces so that the levitated object remains in the same position. Stability is crucial in levitation but difficult to achieve, for this reason many systems need a feedback system (and therefore an additional energy input to the system) that changes dynamically the restoring force. This is called active levitation. Conversely if the restoring force does not need for a feedback system the system is called passive. Some systems start to levitate when the levitating object moves. In this case the levitation is called dynamic levitation, and static otherwise. A good example of dynamic levitation is the levitron1 in which a small spinning magnet levitates over a larger one. In magnetic levitation the force that makes the object to levitate is magnetic. The first levitating system one may think of consist of a magnet placed above a fixed array of magnets. Is it possible to find an array configuration so that the magnet above can levitate static and passively? The answer is negative, the free magnet will wind up attached to the others. More generally, Earnshaw [51] proved mathematically that stable and static levitation is impossible for a body placed in a repulsive or attractive static force field in which the force is dependent on the inverse square of the distance, which is the case of magnetostatic force. In spite of the difficulty in achieving static and passive levitation with magnetic fields, there are some systems in which the Earnshaw theorem can be circumvented [52] using diamagnetic materials or superconductors as explained in the following section.. 2.2. Levitation with Diamagnets and Hard Type II Superconductors. Stable and static levitation with diamagnets is possible because they repel the magnetic field. Levitation of living organisms, that due to their water composition are weakly diamagnetic, has been largely demonstrated. For instance, in Refs. [53, 54] a frog is levitated in a large magnetic field gradient produced by two coils. In biological sciences different techniques [55] have been developed to study the effect of ingravity on cells and plants. Even more surprising is the demonstration of the movement control of single cells [56] due to the field gradient produced by domain walls in ferromagnets. Diamagnets as levitating objects are only stable if placed in local field minimum [54]. Hard type II superconductors however, can achieve levitation not necessarily in a field minimum. When cooling the superconductor below its critical temperature in an arbitrary (static and non uniform) magnetic field distribution, the superconductor remains stuck in the air as if it was in a medium with a lot of friction [57]. This frictional force requires an energy dissipation that is caused by the pinning of the superconducting 1. Commercially available at http://www.levitron.com/.

(27) 2.2 Levitation with Diamagnets and Hard Type II Superconductors. 25. vortices. This fact makes hard type II superconductors good candidates to achieve static and passive levitation because it is possible to make them levitate over an arbitrary arrangement of permanent magnets. Hard type II superconductors also present a large levitation force compared to typical diamagnets because its magnetic response is much more large. This property along with the intrinsic stability of hard type II superconductors is used to levitate heavy systems. Some examples of this are linear magnetic bearings [58] or spaceship propulsion systems [59] but the main applicability is on transportation systems based on superconductors. Since the first demonstration of a man loading levitating vehicle based on this technology [60], projects in China [61], Germany [62] and Brazil [63] have been developing new technology to improve both stability and levitating force of the vehicle. Transportation systems based on hard superconductors usually consist of a guideway of permanent magnets and an array of hard type II superconductors attached to the vehicle. These permanent magnets are made of rare earth materials and have a very large coercivity and high saturation magnetization so that to make a large magnetic field above the guideway. Rare earth price has been soaring for the last few years [64], for this reason some test lines [65, 66, 67] include soft ferromagnets (commonly iron) between the permanent magnets. Soft ferromagnets are also useful to guide the magnetic field of the permanent magnets towards the superconductor and increase its levitation force..

(28)

(29) CHAPTER. 3. Numerical Model for Magnetic Interaction between SC and FM. In this chapter the mathematical model that describes the magnetic behavior of a superconductor and a soft ferromagnet is described. Such a model will also take into account the mutual interaction of both magnetic elements. Different theoretical approaches have been proposed to understand the effects that a soft ferromagnet produces to a superconductor. Many of them use finite element methods assuming linear [68, 69] or non-linear [70] permeability in the ferromagnetic parts. Other authors have obtained analytical results by considering the SC as a perfect diamagnet and an ideal soft ferromagnet (χ → ∞) [71] or image methods considering a finite susceptibility [72] in the ferromagnetic materials. Apart from finite element methods, there are also works based on energy minimization of the SC parts considering linear ferromagnetic materials [73] and others that minimize the energy of the ferromagnetic material combined with iterative methods in the superconductor [74]. Our model assumes a SC in the critical state and an ideal soft ferromagnet both translationally symmetric along the same direction. This model allows the simultaneous calculation of the current profiles in the SC and magnetic pole density in the FM by considering their mutual magnetic interaction and their interaction with an external applied field.. 3.1. Geometry and Magnetic Elements. We consider a FM and a SC, both infinitely long (translationally symmetric) in the z direction and with rectangular cross section of aSC × bSC for the SC (in the x and y directions, respectively) while the FM cross section occupies −aFM /2 ≤ x ≤ aFM /2 in the horizontal direction and −bFM ≤ y ≤ 0 in the vertical direction. Although here we have considered rectangular elements, the model presented is valid for any cross27.

(30) 28. Numerical Model for Magnetic Interaction between SC and FM. sectional shape as long as both elements are infinitely long. An external magnetic field with translational symmetry He (x, y) and no z component is applied to such elements. The SC is assumed to be in the critical-state regime [17, 18]. In general, the criticalcurrent density Jc is field dependent [75] and could be considered in our model by means of iterative methods. However in the present work will always consider Jc independent of the field. The critical current is also temperature dependent but we assume that our simulations are performed at constant temperature and therefore at a fixed Jc . The FM is considered ideal [71], this is, we consider a linear, isotropic and homogeneous FM with a very large value of susceptibility (χ → ∞). This implies that there are only magnetic poles in the surfaces of the ferromagnet and a vanishing total magnetic field H inside it. By construction of the model, we are implicitly assuming that saturation magnetization can never be achieved.. 3.2. Interaction Functional. In this section we describe a functional related to the magnetic energy of the FM and SC. The minimization of this functional will give the physical value of the magnetic pole density distribution in the FM and supercurrents in the SC. Different functionals have been proposed in the literature [76, 77, 78, 79, 80, 81, 82, 83] to find the induced current distribution on the SC in a translational field, those in refs. [80, 81, 83, 84] for instance are based on the energy as the quantity to be minimized. Our functional is an extension of the one presented in [84]. The current density distribution J(r) on the SC volume and the magnetic charge per unit length (surface magnetic pole density) σ(r) on the FM surface at a certain time is obtained by minimizing the functional F [J, σ] = FSC [J, σ] + FFM [J, σ] ,. (3.1). where Z Z Z 1 FSC [J, σ] = J(r)AJ (r)dS − J(r)AJˆ(r)dS + J(r)(Ae (r) − Aˆe (r))dS 2 S S S Z + J(r)(Aσ (r) − Aˆσˆ (r))dS, (3.2) S Z Z Z FFM [J, σ] 1 = σ(r)φσ (r)dl − σ(r)φσˆ (r)dl + σ(r)(φe (r) − φˆe (r))dl µ0 2 l l Z l + σ(r)(φJ (r) − φˆJˆ(r))dl. (3.3) l. Here, dS is the differential of area in the transverse section S of the SC whilst dl is the differential of length in the perimeter l of the transverse area of the FM. The term FSC [J, σ] takes into account the interaction of the currents in the SC with themselves (first and second terms), with an external applied field (third term) and with the FM (last term) whereas the term FFM [J, σ] is the analogous functional for the FM. In Eqs..

(31) 3.2 Interaction Functional. 29. (3.2) and (3.3) A stands for the vector potential, φ for the magnetic scalar potential and the subindexes indicate the source, which can be the external applied field e, the supercurrents J in the SC or the magnetic poles σ in the FM. The hat terms represent the quantities in the previous time layer, therefore Jˆ and σ ˆ are the current densities in the SC and magnetic pole densities in the FM that minimize the functional (3.1) in the previous time1 . The constraints applied to the magnitudes describing the SC and the FM are different. For the SC we impose the critical-state condition [17] which is |J| ≤ Jc . We choose the Coulomb gauge so that the potential vector direction is parallel to the current. In the SC a transport current can be considered when minimizing the functional [82] however in the present work we only consider changes in the SC currents due to external magnetic fields, in this case, the net current in a transverse section of the SC is zero, R R S JdS = 0. For the FM the only constraint needed is l σ(r)dl = 0 indicating that no net magnetic charges are induced. The functional F [J, σ] has units of energy per unit length since the term for the SC (FM) depends on a current density (a magnetic pole density) multiplied by a vector potential (magnetic scalar potential). The first term FSC [J, σ] cannot be considered as simply the energy per unit length of the SC system since it describes a hysteretic process. FSC [J, σ] reduces to the functional introduced by Prigozhin [77, 85] if the interaction with the FM is not considered, i.e., σ(r) is set to zero. Only under some conditions [82] this functional is equivalent to the magnetic energy. The second term FFM [J, σ], however, is µ0 times the energy per unit length of the FM if J(r) is zero, this is so because the FM is non hysteretic. By setting the hat terms in FFM [J, σ] to zero we recover the functional in [74] in which the behavior of a FM substrate was analyzed by just minimizing the energy of the FM. Defining the surface magnetic pole density variation δσ ≡ σ − σ ˆ and current density variation δJ ≡ J − Jˆ it is possible to obtain another functional F0 [δJ, δσ] whose minimization is equivalent to minimize F [J, σ]. So, we define F0 [δJ, δσ] = F0 SC [δJ, δσ] + F0 FM [δJ, δσ] ,. (3.4). where F0 SC [δJ, δσ] =. 1 2 Z. Z. Z δJ(r)AδJ (r)dS +. S. δJ(r)(Ae (r) − Aˆe (r))dS. S. δJ(r)(Aσˆ (r) − Aˆσˆ (r))dS Z Z ˆ + δJ(r)Aδσ (r)dS + J(r)A δσ (r)dS +. S. S 1. (3.5). S. This time dependence can be introduced either by considering an external applied field which changes with time, or by considering that the external applied field is static and the SC and/or the FM are moved relative to the source of magnetic field. With this latter consideration the external applied field varies with time from the standpoint of the SC and/or the FM. In any case variations are performed quasiestatically..

(32) 30. Numerical Model for Magnetic Interaction between SC and FM. and F0 FM [δJ, δσ] µ0. Z Z 1 = δσ(r)φδσ (r)dl + δσ(r)(φe (r) − φˆe (r))dl 2 l l Z δσ(r)(φJˆ(r) − φˆJˆ(r))dl + l Z Z ˆ (r)φδJ (r)dl. δσ(r)φδJ (r)dl + σ +. (3.6). l. l. If σ = δσ + σ ˆ and J = δJ + Jˆ are introduced in F [J, σ], we obtain F0 [δJ, δσ] and other terms that only depend on Jˆ and σ ˆ . Because of the definition of Jˆ and σ ˆ , the terms including only them are already minimized and thus are omitted in Eq. (3.4).. 3.3. Calculation of Currents and Magnetic Poles. The magnetic behavior of the SC and FM is determined by the supercurrents induced in the former and the magnetic pole density originated in the surface of the latter. In this section we show how to calculate both using the functional (3.4) when they are set in a non-uniform applied field with translational symmetry along the z direction. Since the currents in the SC are distributed in its cross section we divide it in NSC rectangular-sectioned elements of infinite length and the same cross sectional area ∆x × ∆y = ∆S. The current density at each element is assumed to be uniform and with a value mJc /mm where mm is a positive integer and m is an integer between −mm and mm . The FM surface is discretized in NFM elements of the same width ∆L and infinite length. In each FM element it is assumed a uniform magnetic pole density that can be ±n∆σ where n is a positive integer with arbitrarily high value. The change of F0 FM [δJ, δσ] due to a magnetic pole density variation ∆σ over the j element of the FM is ∆F0 FM,j µ0. = ∆σ∆L. N FM X p=1. + ∆σ∆L. +. N SC X. k=1 N N FM X SC X. h i 1 Epj δσp + Ejj (∆σ)2 ∆L + ∆σ∆L Ye,j − Yˆe,j 2 N SC X ˆ SC + ∆σ∆L δJk QSC Jˆk QSC − Q kj kj kj. σˆp δJk QSC kp ∆L,. k=1. (3.7). p=1 k=1. where Epj and QSC kj are related to the magnetic scalar potential at the j element of the SC due to a p element of the FM and a k element of the SC, respectively. These quantities are geometrical factors between the element j of the SC and another element of the FM or SC and are defined and explained in Sec. A.1 of Appendix A. Ye,j is the magnetic scalar potential at the center of an element j in the FM due to an external ˆ SC applied field (He ). The quantity QSC kj − Qkj is related to the change in magnetic scalar.

(33) 3.3 Calculation of Currents and Magnetic Poles. 31. potential at an element j of the FM due to a change in the relative positions between j and an element k in the SC with respect to the previous time layer. We can perform the equivalent change of current ∆I in an element i of the SC that leads to a variation of the functional F0 SC [δJ, δσ] by an amount. ∆F0 SC,i µ0. = ∆S∆I. + ∆I. N SC X. h i 1 ˆ e,i Dki δJk + Dii (∆I)2 + ∆I Ge,i − G 2. k=1 N FM X. σ ˆp. QFM pi. N FM X FM ˆ − Qpi + ∆I δσp QFM pi. p=1. +. N SC N FM X X. p=1. Jˆk δσp QFM pk ∆S,. (3.8). k=1 p=1. where Dki and QFM pi are quantities related to the magnetic vector potential over an element i of the SC created by a k element of the SC and a p element of the FM, respectively. As above, the first two quantities are geometrical factors between the element i and another element of the FM or SC, further explanation and exact calculation of Dki and QFM pi can be found in Appendix A Sec. A.2. Ge,i is the magnetic vector potential per ˆ FM unit µ0 due to an external applied field (He ). In the third term the quantity QFM pi − Qpi takes into account the change of magnetic vector potential at the i element of the SC produced by a p element of FM due to a change in the relative position between i and p in the previous and present time layer. For a given current density Jˆ and magnetic pole density σ ˆ distributions (both are zero at the beginning) we calculate the next values of J and σ on the new field characterized by Ae and φe by minimizing the sum of the two discretized functionals of Eqs. (3.8) and (3.7) in the following way. First we consider ∆σ = 0, hence the functional Eq. (3.7) is zero except the last term, and we find the pair of elements in the SC such that by setting a current increment ∆I = ∆SJc /mm and −∆I, respectively, the sum of the two functionals would decrease the most but always keeping the condition |J| ≤ Jc fulfilled. In the same way, we consider ∆I = 0, and so the functional Eq. (3.8) becomes zero except the last term. We then find the pair of elements in the FM for which an increment of magnetic pole density ∆σ and −∆σ, respectively, would decrease the sum of the two functionals the most. Once the pair of currents and magnetic pole densities are found we choose the pair (either of currents or magnetic poles) that minimizes the most the sum of the functionals. This pair of poles or currents are added to their respective discretization elements. This step of minimization is repeated until the sum of the functionals can not be further minimized. In the process of finding the optimum pair the last term of both Eqs. (3.7) and (3.8) are not considered since they are additive constants independently of the trial-position for ∆I and ∆σ..

(34) 32. 3.4. Numerical Model for Magnetic Interaction between SC and FM. Calculation of Levitation Force. In the case of magnetic levitation, we are interested in obtaining the magnetic force over the SC. This force comes from the interaction of the currents in the SC and the magnetic field Hm produced by the guideway (FMs and PMs), i.e. it is a Lorentz force. Once we obtain the current distribution in the SC and the magnetic pole density in the FM the vertical force per unit length L exhibited by the SC is Z Fy (3.9) = µ0 Jz Hm, x dS, L S where Jz is the current density, S is the cross section of the SC and Hm, x is the xcomponent of the magnetic field created by the guideway (PMs and FM) at the crosssection of the SC. Similarly, horizontal force (guidance force) per unit length is Z Fx (3.10) = −µ0 Jz Hm, y dS, L S where Hm, y is the y-component of the magnetic field created by the guideway over the SC. In our model, the SC cross section is discretized and Eqs. (3.9) and (3.10) can be approximated as Fy L Fx L. ' µ0. N SC X. Hm, x, j Ij ,. (3.11). j=1. ' −µ0. N SC X. Hm, y, j Ij ,. (3.12). j=1. respectively. In these two equations Ij = Jj ∆S is the current at the j-element and Hm, x, j , Hm, y, j are the horizontal and vertical components of the field created by the guideway in the center of the element j of the SC.. 3.5. Calculation of Stability. In levitation systems it is not only important the force acting on the levitating body (in our case the SC) but the restoring forces over it when the body undergoes small displacements around its equilibrium position. The vertical and horizontal stiffnesses per unit length are defined as κyy L κxx L. ∂Fy /L , ∂y ∂Fx /L = − , ∂x = −. (3.13) (3.14). respectively. For the system to be stable, vertical and horizontal stiffnesses must remain positive around the levitation point..

(35) 3.6 Limits and Validity of the Model. 3.6. 33. Limits and Validity of the Model. The SC is assumed to be below its critical temperature Tcrit (around 77K for YBCO) whilst the FM is below its Curie temperature Tc [7] which is typically 1044K for iron [2]. Our simulations are performed in a quasi-static situation. The approximation of considering the soft ferromagnet as a perfect soft ferromagnet is justified by the large susceptibilities (χ ∼ 105 − 106 ) and very low coercivities (Hc ∼ 1 − 10 A/m) found in some magnetic materials manufactured today [2, 86, 87]. These ferromagnets are smartly located in electromagnets, transformers or motors where low coercivities and large susceptibilities are advisable [2]. All these materials get saturated when set in a sufficiently large applied field. In our model the saturation of the soft ferromagnet is not considered. This may restrict ourselves to simulations where magnetic fields are not large. However, even in this case our model can give a first approximation..

(36)

(37) CHAPTER. 4. Magnetic Response of an Ideal Soft Ferromagnet. Before analyzing the mutual interaction between the SC and FM in the levitation case, it is important to understand the magnetic behavior of both SC and FM separated. The simplest case is to submit the FM or SC to a constant applied field. The SC response to a uniform applied field has already been studied for different geometries, such as slabs [17], or infinitely long bars with rectangular [88, 89, 90] or elliptical [91, 92] cross sections among others [27]. Also, much research has been done when the applied field over the SC is non-uniform [27, 93, 95]. However no systematic study of a FM under different applied fields has been carried out. In this chapter we analyze the magnetic response of the FM bar set in a uniform applied field or a field produced by PMs, i.e. non-uniform.. 4.1. Uniform Applied Field. The simplest case is to consider a FM immersed in a uniform applied field. Studying this case not only allows us to understand the basic behavior of the FM but also to validate our results through analytical calculations. In our case of translationally symmetric ideal soft ferromagnet with rectangular cross section aFM × bFM there exists an analytical solution for the magnetic pole density distribution at its surface [96]. In our simulation, we consider a vertical applied field (perpendicular to aFM side) ˆ , where Ha is positive (see inset of Fig. 4.1). Figure 4.1 shows the distribution He = Ha y of surface magnetic pole density in the FM for several values of bFM /aFM obtained by numerical calculations (symbols) and by the analytical expressions of the Ref. [96] (lines). We will refer to the different sides of the FM as top (T, y = 0), bottom (B, y = −bFM ), left (L, x = −aFM /2) and right (R, x = aFM /2). For sake of simplicity only the pole densities of the upper right corner are plotted since, in the uniform applied field case, the pole distribution is horizontally symmetric and vertically antisymmetric 35.

(38) 36. Magnetic Response of an Ideal Soft Ferromagnet. b. F M. /a. F M. b. F M. /a. F M. b. F M. /a. F M. 5. 4. R. T. = 1 = 1 0. / H. a. 3. = 0 .1. b 2. Y. T L. X. F M. B. 1. H. a. Z. R F M. a. 0 x = a. F M. /2 , y = -b. F M. /2. x = a. F M. /2 , y = 0. x = 0 , y = 0. Figure 4.1: Comparison of the numerical (symbols) and analytical (lines) distributions of surface magnetic pole density of a FM set in a uniform applied field in the positive y direction for different ratios bFM /aFM . The inset shows an sketch of the considered system. Because of the symmetry, on the abscissa only the position of poles starting from the middle of the right side (R) to the middle of the top side (T) are represented counterclockwise (see blue line and the arrow in the inset).. with respect to the center of the FM (x = 0,y = −bPM /2). By comparing numerical and analytical distributions we can see that there is an excellent agreement between both, so the validity of our model in this limit is confirmed. To make the total field H zero inside, the FM has to produce a negative vertical component of magnetic field in its interior. For this reason top and bottom sides must have positive and negative values of magnetic pole density, respectively. As can be seen in Fig. 4.1 these sides have a quasi-constant magnetic pole density at the regions far from the corners. This distribution creates a quasi-uniform vertical magnetic field in the central region in order to cancel the applied field. Near the corners however, a uniform magnetic pole density can no longer exist, otherwise a large horizontal field would be created in the interior region near the corners. Istead, the magnetic pole density increases in all the sides near the corners so that the horizontal field is completely canceled. Magnetic pole density diverges in the corners as can be seen in Fig. 4.1. Top and bottom sides diverge more rapidly than left and right side do, to make a net field in the -y direction. This is, if both sides were to diverge in the same way, their field would cancel mutually and therefore near the corners we would not have a zero total field. The linearity of the FM is evidenced in Fig. 4.1 (see the normalization of σ). For the same FM, if the applied field is changed by a factor, the magnetic pole density at each point will be multiplied by the same factor. Since the applied field has the same.

(39) 4.2 Permanent-Magnet field. 37. value and direction at every point in the space, the magnetic pole density shape and value for a given applied field only depend on the aspect ratio bFM /aFM . It is interesting to see that when bFM /aFM << 1 we can approximate the top and bottom sides in a region far from the corners as two uniformly charged infinite sheets. As said previously, these distributions produce a quasi uniform vertical field inside the sample. In this case, the magnetic pole density is |σ| = Ha far from the corners (see red curve in Fig. 4.1). By contrast, when bFM /aFM >> 1 the absolute value of pole density of the top and bottom sides increases (black curve in Fig. 4.1) and tends to diverge. A simple explanation can be given looking at the central point of the FM (x = 0, y = −b/2). Since top and bottom sides are farther from this point when bFM /aFM increases they must increase their magnetic pole density to make the same vertical field and cancel the applied field.. 4.2. Permanent-Magnet field. We now move to a case where the applied field is not uniform, as for example the field created by a square-sectioned PM. The FM is placed just above the PM, which is uniformly magnetized in the y direction (MPM = 7.95 × 105 A/m) and of side aPM = 0.1 m. In this way the bottom side of the FM is always in contact with the top side of the PM. In this example, as opposed to the case of a uniform applied field, the shape of the magnetic pole density depends on the ratios aFM /aPM and bFM /aPM . Changing the side lengths of the FM while keeping its aspect ratio fixed changes the magnetic pole density shape because the field felt by each side also changes. For the case of a square-sectioned FM with the same side as the PM (aFM = bFM = aPM ) we find the magnetic pole distribution of Fig. 4.2(a) when the field is created by the PM (dashed line) compared to the response to a uniform applied field as in the previous section (line). In the case of the PM field, the surface pole density σ is normalized to HPM , which is defined as the magnetic field created by a PM of square cross section at the center of its surface perpendicular to the magnetization (HPM ' 0.35M ). In the case of the uniform applied field, σ is normalized to Ha . Figure 4.2(a) shows that, unlike the case with uniform applied field, all surfaces of the FM have positive density except the bottom one. This result can be understood by looking at Fig. 4.2(b) where the magnetic field lines produced by the PM are represented. In these profiles we find that the PM field tends to enter from the bottom side of the FM and exit through the rest of the sides. Furthermore, the non uniformity of the PM field is responsible for the difference, in modulus, between the poles of the upper and lower surfaces. The shape of the pole distribution in the bottom surface also creates a negative horizontal field in the region x > 0 and positive in x < 0 which compensates the horizontal field produced by the PM in this surface [see Fig. 4.2(b)]. Finally, in Fig. 4.2(a) it can be seen that left and right surfaces have a large positive value of magnetic pole density near the PM (y ≈ −bFM ).

(40) 38. Magnetic Response of an Ideal Soft Ferromagnet. (b ). (a ) 6 4. , σ/ H. P M. 2. σ/H. a. 0 -2 T. L. -4. F M. F M. F M. R. F M. B. -6. Figure 4.2: (a) Magnetic pole density of a square-sectioned FM of side aFM = 0.1 m set in a uniform applied field Ha (line) and in a field produced by a PM (dashed line). The PM has the same square cross section as the FM and is uniformly magnetized in the positive y direction with a saturation magnetization MPM = 7.95 × 105 A/m. Magnetic pole densities are normalized to the applied field and HPM (see text). The positions of magnetic pole density are represented on the abscissa starting from the left (L) surface of the FM and then following counterclockwise the bottom (B), right(R) and top (T) surfaces. (b) Calculated magnetic field lines produced by only the PM. The position of the FM is marked with a dashed square on top of the PM.. and this value decreases as the pole approaches to the top side because the horizontal field produced by the PM in the lateral sides is higher near the PM. It should be noted that the sign and value of magnetic pole density at each point of the FM surface does not only depend on the external magnetic field at a particular point but on the field of all the other poles in that point. Analyzing the behavior of all magnetic poles can be cumbersome, therefore, we focus now on a single pole as representative of the overall response. In Fig. 4.3 we plot how the pole density at the center of the top side (x = 0) varies for three different heights of the FM (bFM ) as a function of its width (aFM ) being the PM kept always the same as before. The dependence of the top central pole density with the FM width is, in general, very similar in the three studied heights, i.e., the pole density increases for small widths and it decreases when the FM is widened. For a fixed aFM , the case of the thin FM (bFM /aPM = 0.5) is the one that provides larger central pole density since the thinner the FM is the stronger the field felt by the top side is because of its closeness to the PM. When the width of the FM is very large (aFM → ∞) the central magnetic pole density at the FM top side tends to zero for all bFM ’s. In fact, this result is extended to all poles of the upper surface. In the bottom surface, however, magnetic pole density at each point tends to double the value of the vertical component of the PM field at the particular point. One way to understand these results is to apply the image method [3, 97, 98], approximately valid in this limit because the FM volume and in particular its bottom surface are equipotential. The sum of the field produced by the PM and.

(41) 4.2 Permanent-Magnet field. 39. 0 .2 5. a. F M. /a. P M. b. = 1 /3 b b. 0 .2 0. a. /a. F M. a. 0 .1 5. P M. P M. b. F M F M. /a /a /a. P M P M P M. = 0 .5 = 1 = 2. = 2 a. F M. b. / M. F M. F M. F M. /a. P M. = 5. P M. 0 .1 0 a. P M. 0 .0 5. 0 .0 0 0 .0. 0 .5. 1 .0. 1 .5. 2 .0. 2 .5. a. 3 .0 F M. /a. 3 .5. 4 .0. 4 .5. 5 .0. 5 .5. 6 .0. P M. Figure 4.3: Magnetic pole density in the middle of the top side of the FM (marked with ×) as a function of the FM width (aFM ) for different heights (bFM ). Black line, red dashed line and blue dotted line represent the ratios bFM /aPM = 0.5, 1, 2, respectively. The corresponding straight lines represent the vertical field produced by the PM at the same points of the FM for the different curves bFM /aPM . The pole density σ is normalized to the PM magnetization MPM . The insets are sketches of the geometry for the curve bFM /aPM = 0.5 and three values of aFM . its image will be the total magnetic field in the region y ≤ −bFM (under the FM). On the bottom side of the FM this sum is twice the field created by one of the PMs, and therefore σ is twice the vertical component of the PM field in this surface. In this limit, since the bottom side completely cancels the field produced by the PM for the region y > −bFM (inside the FM and above it) there is no need for the top side to cancel any field and thus its pole density is zero. By contrast, when the width of the FM is very small (aFM → 0) for a fixed bFM the magnetic pole density in the middle of the FM top surface diverges, because since the width shrinks, there is less surface able to create a field capable to cancel the PM field and so the top and bottom parts must have a large magnetic pole density. FMs are added to PMs systems in order to modify the total magnetic field at some points without the need to increase the number of PMs. For this purpose in Fig. 4.3 it is also represented the magnetic field produced by the PM in the middle of the top side (straight black, red dashed and blue dotted lines for bFM /aFM =0.5,1,2, respectively). Figure 4.3 shows that, in the studied point, the set FM-PM generates more magnetic field than the case of a single PM when the width of the FM is small and the opposite happens when the width is large. Therefore, using a FM does not always enhance the.

(42) 40. Magnetic Response of an Ideal Soft Ferromagnet. magnetic field at a given point of interest. The shape of the FM is a crucial parameter. In particular, as the height of the FM increases the range of aFM /aPM at which the magnetic field is enhanced also increases.. 4.3. Two Permanent-Magnets Field. A more sophisticated case is when the applied field is produced by two squaresectioned PMs which are the same saturation magnetization MPM and side aPM as in the previous section. These two PMs are attached to the left and right sides of the FM (see inset of Fig. 4.4) with magnetizations in the positive and negative horizontal directions, respectively. The top sides of the three elements, PMs and FM are kept vertically aligned at y = 0. As it will be seen in the next chapter, this geometry is particularly interesting for levitation for it produces a large vertical and horizontal fields above it. 3. b 2. L F M. /a. B. R. T P M. F M. v e r tic a l fie ld. 1 .0 0 .8 0 .6 0 .4 0 .2 1. / M. P M. 0 0 .3 2. -1. -2. P M. 0 .2 6. y. 0 .2 8. / M , H. F M. /M. 0 .3 0. 0 .2 4 0 .2 2 0 .2 0 0 .1 8. -3. Figure 4.4: Distribution of magnetic pole density of a FM of width aFM = aPM and different heights (bFM ) set between two square-sectioned PMs with antiparallel magnetization in the x direction. On the abscissa the positions of the pole densities are represented starting from the left (L) surface and then the bottom (B), right (R) and top (T) surfaces, successively. The left inset shows an sketch of the guideway with bFM /aFM = 0.6. The right inset shows a zoom of the central region of the FM top surface. Orange dashed dot dot line is the vertical field produced by only the two PMs in the top side of the FM.. The magnetic pole density of the FM surface for different FM heights bFM is shown in Fig. 4.4. In the case of the square FM (black line), the sign of the magnetic pole density is positive for the top and bottom sides (where the PM field tends to exit the FM) and negative in the left and right sides (where the PM field tends to enter the FM). The reason is that the FM tends to cancel the field perpendicular at each side..

(43) 4.3 Two Permanent-Magnets Field. 41. According to this, the magnetic pole density in the top and bottom sides is maximum near the corners and minimum towards the middle (x = 0), as seen in Fig. 4.4, because the vertical component of the field produced by the PMs is larger near the corners. By contrast, the absolute value of magnetic pole density in the left and right sides takes its maximum in the middle of the side (y = −bPM /2) since the field perpendicular to this side produced by the PMs is maximum in this point and decreases towards the edges. When the height of the FM changes, the field produced by the PMs over each point in the surface of the left, right and bottom parts also changes. More specifically, as the height of the FM decreases, two negatively charged regions appear in the bottom side close to the edges (see Fig. 4.4). For small heights, these regions extend and eventually occupy the entire lower surface. This behavior is consequence of three effects. The first one is that the vertical PM field begins to enter through the bottom surface when bFM < aPM /2, so the bottom part tends to be negative as the FM is shrunk. The second effect is due to the increase of the negative magnetic pole density on the lateral sides close to the bottom. This makes a positive vertical field over the region of the bottom part close to the left and right sides and thus more negative magnetic pole density builds up. Finally, the third effect comes from the positive top side, which tends to make a large negative vertical field over the bottom side as the height of the FM is shrunk. This makes the poles of the bottom side to decrease.. Figure 4.5: Magnetic field lines above the system of two square-sectioned PMs (aPM = bPM = 0.1 m) uniformly magnetized in opposite directions of x pointing each other (black dashed lines) and the same system with a FM width of aPM and height of bFM /aPM = 0.6 set in the middle of the two PMs (red solid lines). We find that the largest value of the magnetic pole density over the whole top side at a ratio bFM /aPM = 0.66 (Fig. 4.4). This is because the magnetic pole density over the top side depends mostly on the field produced by the bottom side over the upper one..

(44) 42. Magnetic Response of an Ideal Soft Ferromagnet. Particularly, it depends on the relative distance between top and bottom sides and the sign of the poles of the latter. As the FM height is shrunk from bFM = aFM , magnetic field over the top side produced by the bottom one increases because the latter side is positively charged. Therefore, the magnetic pole density increases in the top side (see inset of Fig. 4.4). However, the bottom side becomes eventually negatively charged and hence it produces a negative vertical field over the top side. This results in decreasing the magnetic pole density over the top side. The height at which the compensation of both effects occurs is bFM /aPM ≈ 0.66. Although the results of Fig. 4.4 are obtained for a fixed width (aFM = aPM ), when different FM widths are considered, the largest values of the top pole density are also found for similar ratios bFM /aPM , being slightly higher or lower than 0.66 when the width increases or decreases, respectively. Since the field at any point in the surface is perpendicular to it and with the value of the magnetic pole density, poles in the top surface indicate the vertical field just above the FM. Comparing to the vertical field produced by the two PMs (orange dashed dot dot curve in Fig. 4.4) we see that in fact any FM improves the vertical field above the guideway but for bFM /aPM ≈ 0.66 this field is the highest. Magnetic pole density over the FM not only indicates the strength of the vertical field but of the horizontal field and its effect can be thought of as a uniformly charged sheet for a first approximation. We compare magnetic field lines with FM (bFM /aPM ≈ 0.66) and without it in Fig. 4.5. As it can be seen, field lines are closer when the FM is present, indicating a larger field.. 4.4. Chapter Summary and Conclusions. The magnetic response of a soft ferromagnetic bar has been studied in different applied fields. A remarkable agreement between our calculations and the previously analytical results has been found. In the cases of non-uniform applied field we have seen how by tuning the shape of the FM we can change the field at the FM surroundings. Special focus has been given to the case of an ideal soft ferromagnet set between two permanent magnets. We have determined that when the two PMs are square-sectioned, a good option to maximize the field above them is to set a soft FM in between with height approximately 0.6 times the height of the PMs. This result can be useful when designing magnetic levitation trains based on superconducting levitation..

Outline

Related documents

The space or region around a magnet or a current carrying conductor in which its influence can be felt by any magnetic substance is called magnetic field.. Magnetic field

The WFIS OCIP Administrator will provide a Certificate of Insurance evidencing workers’ compensation & employer’s liability, general liability, and excess

This figure reports the average standard deviation of holding period returns net of fees of 25,000 randomly chosen portfolios ranging from two to 350 underlying hedge funds

§ Students are expected to abide by the Student Code of Conduct and the Scholastic Code of Conduct found in the Eastern Arizona College Student Handbook.. Copies are available at

A moving charge or a electric current produces a magnetic field in the surrounding space (It also produces an electric field).. The magnetic field exerts a force on any other

Hence, by the interaction between the magnetic field and the eddy current field, the rotary torque and the linear force will be produced to drive the mover to do

The underlying expectation of using reconstruction loss for OoD detection is that since generative models learn to generate images based on the in-distribution data, they should be

Capacitor – energy of a charged capacitor - loss of energy due to sharing of charges – magnetic field due to a current carrying conductor – Biot Savart’s Law – Field along the